Fluorescent Tryptophan-Doped Silica Microparticles
Prepared Through a Reverse Microemulsion Method
Janine Marriah G. Dela Cruz1,2 and Christopher Jay T. Robidillo1*
1Department of Physical Sciences and Mathematics
College of Arts and Sciences, University of the Philippines Manila
2College of Medicine, University of the Philippines Manila
A reverse microemulsion method was utilized in synthesizing silica microparticles doped with tryptophan molecules as fluorophore. The fluorescent microparticles were formed inside reverse micelles dispersed in a cyclohexane continuous phase. The microparticles were produced within 24 hours and showed strong emission at a wavelength of 285 nm. The blue shift in their fluorescence maximum can be attributed to the caging and confinement effects of the silica network on the encapsulated tryptophan molecules. Successful encapsulation of tryptophan was confirmed through Fourier Transform Infrared Spectroscopy and Energy-Dispersive X-Ray Spectroscopy. Scanning Electron Microscopy and Dynamic Light Scattering Analysis revealed that the diameters of tryptophan-doped silica microparticles were in the range of 203 to 692 nm in the solid state, and in the range of 223 to 341 nm, with a narrow size distribution centered at 282 nm, in aqueous solution. Properties relevant to probe applications such as photostability and fluorophore leakage were also investigated. Tryptophan-doped silica microparticles were found to maintain their photostability even after six hours of continuous exposure to a 150 W halogen lamp and were observed to not undergo tryptophan leakage after three days of aqueous dispersion. This study has effectively extended dye encapsulation in silica to a biologically endogenous fluorescent amino acid, yielding fluorescent microparticles with desirable properties for fluorescent probes, namely, biocompatibility, photostability, non-leakage, monodispersity in solution, and fairly uniform sizes.
Fluorescence spectroscopy is a luminescent technique that has gained considerable interest due to its ease of implementation, and high sensitivity and selectivity. Innovations in fluorescent analytical techniques have been applied in the development of sensors for probing chemical and biological processes (Basabe-Desmonts et al. 2006). These probes were successfully used in biological research, clinical diagnosis, and detection of various kinds of substances (Lian et al. 2004; Liaud et al. 2015; Liu et al. 2015; Hodáková et al. 2015; Qin et al. 2016). . . . read more
AVNIR D, LEVY D, REISFELD R. 1984. The nature of the silica cage as reflected by spectral changes and enhanced photostability of trapped rhodamine 6G. Journal of Physical Chemistry 88(24):5956-5959.
AUGER A, SAMUEL J, PONCELET O, RACCURT O. 2011. A comparative study of non-covalent encapsulation methods for organic dyes into silica nanoparticles. Nanoscale Research Letters 6(328):1-12.
BAGWE RP, YANG C, HILLIARD LR, TAN W. 2004. Optimization of dye-doped silica nanoparticles prepared using a reverse microemulsion method. Langmuir 20:8336-8342.
BALAURE PC, POPA RA, GRUMEZESCU AM, VOICU G, RADULESCU M, MOGOANTA L, BALSEANU T, MOGOSANU GD, CHIFIRIUC MC, BLEOTU C, HOLBAN AM, BOLOCAN A. 2016. Biocompatible hybrid silica nanobiocomposites for the efficient delivery of anti-staphylococcal drugs. International Journal of Pharmaceutics 510:532-542.
BARIA MP, NGUYEN E, PACE SJ, MARVIN RL, MOJICA EE. 2014. Spectrochemical behavior of enzymes encapsulated within xerogel. Journal of Physical Chemistry and Biophysics 4:1-4.
BASABE-DESMONTS L, REINHOUDT DN, CREGO-CALAMA M. 2006. Design of fluorescent materials for chemical sensing. Chemical Society Reviews 36(6):993-1017.
BURSTEIN EA, VEDENKINA NS, IVKOVA MN. 1973. Fluorescence and the location of tryptophan residues in protein molecules. Photochemistry and Photobiology 18(4):263-279.
CANTON G, RICCO R, MARINELLO F. 2011. Modified Stober synthesis of highly luminescent dye-doped silica nanoparticles. Journal of Nanoparticle Research 13(9): 4349-4356.
CHANG CL, FOGLER HS. 1997. Controlled formation of silica particles from tetraethyl orthosilicate in nonionic water-in-oil microemulsions. Langmuir 13(13):3295-3307.
CHEN G, SONG F, WANG X, SUN S, FAN J, PENG X. 2012. Bright and stable cy3-encapsulated fluorescent silica nanoparticles with a large Stokes shift. Dyes and Pigments 93(1):1532-1537.
CHEN RF. 1967. Fluorescence quantum yields of tryptophan and tyrosine. Analytical Letters 1(1):35-42.
CHEN Y, BARKLEY MD. 1998. Toward understanding tryptophan fluorescence in proteins. Biochemistry 37(28): 9976-9982.
CHEN ZZ, CAI L, CHEN MY, LIN Y, PANG DW, TANG HW. 2015. Indirect immunofluorescence detection of E. coli O157: H7 with fluorescent silica nanoparticles. Biosensors and Bioelectronics 66:95-102.
FALES AM, YUAN H, VO-DINH T. 2011. Silica-coated gold nanostars for combined SERS detection and singlet oxygen generation: A potential nanoplatform for theranostics. Langmuir 27(19):12186-12190.
FLYNN SP, KELLEHER SM, ACORN JN, KURZBUCH D, DANIELS S, MCDONAGH C, CLANCY E, SMITH TJ, NOONEY R. 2016. Ultrasensitive microarray bioassays using cyanine5 dye-doped silica nanoparticles. Nanotechnology 27(46):465501-465507.
GAO F, TANG L, DAI L, WANG L. 2007. A fluorescence ratiometric nano-pH sensor based on dual fluorophore-doped silica nanoparticles. Spectrochimica Acta Part A 67(2):517-521.
GAO H, ZHAO Y, FU S, LI B, LI M. 2002. Preparation of a novel polymeric fluorescent nanoparticle. Colloid Polymer Science 280(7): 653-660.
GAO X, HE J, DENG L, CAO H. 2009. Synthesis and characterization of functionalized rhodamine B-doped silica nanoparticles. Optical Materials 31(11):1715-1719.
GU J, WANG T, FAN G, MA J, HU W, CAI X. 2016. Biocompatibility of artificial bone based on vancomycin loaded mesoporous silica nanoparticles and calcium sulfate composites. Journal of Materials Science: Materials in Medicine 27(4):1-11.
HODAKOVA J, PREISLER J, FORET F, KUBAN P. 2015. Sensitive determination of glutathione in biological samples by capillary electrophoresis with green (515nm) laser-induced fluorescence detection. Journal of Chromatography A 1391:102-108.
JOUMAA N, TOUSSAY P, LANSALOT M, ELAISSARI A. 2008. Surface modification of iron oxide nanoparticles by a phosphate-based macromonomer and further encapsulation into submicrometer polystyrene particles by miniemulsion polymerization. Journal of Polymer Science Part A: Polymer Chemistry 46(1):327-340.
KABALNOV A, OLSSON U, WENNERSTROEM H. 1995. Salt effects on nonionic microemulsions are driven by adsorption/depletion at the surfactant monolayer. Journal of Physical Chemistry 99(16):6220-6230.
KAHLWEIT M, STREY R, BUSSE G. 1990. Microemulsions: a qualitative thermodynamic approach. Journal of Physical Chemistry 94(10): 3881-3894.
KELLEHER SM, NOONEY RI, FLYNN SP, CLANCY E, BURKE M, DALY S, SMITH TJ, DANIELS S, MCDONAGH C. 2015. Multivalent linkers for improved covalent binding of oligonucleotides to dye-doped silica nanoparticles. Nanotechnology, 26(36): 365703-365714.
LI H, MU Y, QIAN S, LU J, WAN Y, FU G, LIU S. 2015. Synthesis of fluorescent dye-doped silica nanoparticles for target-cell-specific delivery and intracellular MicroRNA imaging. Analyst 140(2): 567-573.
LIAN W, LITHERLAND SA, BADRANE H, TAN W, WU D, BAKER HV, GULIG PA, LIM DV, JIN S. 2004. Ultrasensitive detection of biomolecules with fluorescent dye-doped nanoparticles. Analytical Biochemistry 334(1):135-144.
LIAUD C, MILLET M, LE CALVE S. 2015. An analytical method coupling accelerated solvent extraction and HPLC-fluorescence for the quantification of particle-bound PAHs in indoor air sampled with a 3-stages cascade impactor. Talanta 131:386-394.
LIU J, ZHANG L, WANG Y, LIU G. 2014. Preparation of acridine orange-doped silica nanoparticles for pH measurement. Journal of Luminescence 147:155-158.
LIU Y, LI K, WU MY, LIU YH, XIE YM, YU XQ. 2015. A mitochondria-targeted colorimetric and ratiometric fluorescent probe for biological SO2 derivatives in living cells. Chemical Communications 51(50): 10236-10239.
MILETTO I, GILARDINO A, ZAMBURLIN P, DALMAZZO S, LOVISOLO D, CAPUTO G, VISCARDI G, MARTRA G. 2010. Highly bright and photostable cyanine dye-doped silica nanoparticles for optical imaging: photophysical characterization and cell tests. Dyes and Pigments 84(1):121-127.
MONTALTI M, PRODI L, ZACCHERONI N, BATTISTINI G, MARCUZ S, MANCIN F, RAMPAZZO E, TONELLATO U. 2006. Size effect on the fluorescence properties of dansyl-doped silica nanoparticles. Langmuir 22(13):5877-5881.
NOONEY R, O’CONNELL C, ROY S, BOLAND K, KEEGAN G, KELLEHER S, DANIELS S, MCDONAGH C. 2015. Synthesis and characterisation of far-red fluorescent cyanine dye doped silica nanoparticles using a modified microemulsion method for application in bioassays. Sensors and Actuators B: Chemical 221:470-479.
OH C, CHUNG S, SHIN S, KIM YC, IM S, OH S. 2002. Distribution of macropores in silica nanoparticles prepared by using multiple emulsions. Journal of Colloid and Interface Science 254(1):79-86.
OHTA T, KIMURA M. 1970. Statistical analysis of the base composition of genes using data on the amino acid composition of proteins. Genetics, 64(3-4):387-395.
OW H, LARSON DR, SRIVASTAVA M, BAIRD BA, WEBB WW, WIESNER U. 2005. Bright and stable core-shell fluorescent silica nanoparticles. Nano Letters 5(1):113-117.
PARK JT, SEO JA, AHN SH, KIM JH, KANG SW. 2010. Surface modification of silica nanoparticles with hydrophilic polymers. Journal of Industrial and Engineering Chemistry 16(4):517-522.
QIN W, WANG K, XIAO K, HOU Y, LU W, XU H, WO Y, FENG S, CUI D. 2016. Carcinoembryonic antigen detection with “Handing”-controlled fluorescence spectroscopy using a color matrix for point-of-care applications. Biosensors and Bioelectronics.
REISS H. 1952. The statistical mechanical theory of irreversible condensation. I. Journal of Chemical Physics 20(8):1216-1227.
ROUHANI S, HAGHGOO S. 2015. A novel fluorescence nanosensor based on 1, 8-naphthalimide-thiophene doped silica nanoparticles, and its application to the determination of methamphetamine. Sensors and Actuators B: Chemical 209:957-965.
SANTRA S, ZHANG P, WANG K, TAPEC R, TAN W. 2001. Conjugation of biomolecules with luminophore-doped silica nanoparticles for photostable biomarkers. Analytical Chemistry 73(20):4988-4993.
SHAHABI S, TRECCANI L, REZWAN K. 2015. Amino acid-catalyzed seed regrowth synthesis of photostable high fluorescent silica nanoparticles with tunable sizes for intracellular studies. Journal of Nanoparticle Research 17(6):1-15.
TAN J, YANG N, HU Z, SU J, ZHONG J, YANG Y, YU Y, ZHU J, XUE D, HUANG Y, LAI Z, HUANG Y, LU X, ZHAO Y. 2016. Aptamer-functionalized fluorescent silica nanoparticles for highly sensitive detection of leukemia cells. Nanoscale Research Letters 11(1): 298-305.
TEALE FWJ. 1960. The ultraviolet fluorescence of proteins in neutral solution. Biochemical Journal 76(2):381-388.
VIVIAN JT, CALLIS PR. 2001. Mechanisms of tryptophan fluorescence shifts in proteins. Biophysical Journal 80(5):2093-2109.
WANG L, WANG K, SANTRA S, ZHAO X, HILLIARD LR, SMITH JE, WU Y, TAN W. 2006. Watching silica nanoparticles glow in the biological world. Analytical Chemistry 78(3):646-654.
WOLFBEIS OS. 2015. An overview of nanoparticles commonly used in fluorescent bioimaging. Chemical Society Reviews 44(14):4743-4768.
XU S, HARTVICKSON S, ZHAO JX. 2011. Increasing surface area of silica nanoparticles with a rough surface. ACS Applied Materials and Interfaces 3(6): 1865-1872.
YOKOI T, WAKABAYASHI J, OTSUKA Y, FAN W, IWAMA M, WATANABE R, ARAMAKI K, SHIMOJIMA A, TATSUMI T, OKUBO T. 2009. Mechanism of formation of uniform-sized silica nanospheres catalyzed by basic amino acids. Chemistry of Materials 21(15):3719-3729.
YOO H, PAK J. 2013. Synthesis of highly fluorescent silica nanoparticles in a reverse microemulsion through double-layered doping of organic fluorophores. Journal of Nanoparticle Research 15(5): 1609-1618.
ZHANG Y, HSU BYW, REN C, LI X, WANG, J. 2015. Silica-based nanocapsules: synthesis, structure control and biomedical applications. Chemical Society Reviews 44(1):315-335.